IOSR Journal of Mechanical and Civil Engineering (IOSR-JMCE) e-ISSN: 2278-1684 Volume 6, Issue 1 (Mar. - Apr. 2013), PP 73-82 www.iosrjournals.org

Prediction of Compressive Strength of Sawdust Ash- Cement Concrete Using Osadebe’s Regression Function 1

D.O. Onwuka, 1L.Anyaogu, 1T.U. Anyanwu and 2Chijioke C. 1

Department of Civil Engineering Federal University of Technology, Owerri, Nigeria 2 Department of Civil Engineering Federal Federal Polytechnic Nekede, Owerri, Nigeria

Abstract: This work aims at developing mathematical model for predicting the compressive strength of sawdust ash – cement concrete based on Osadebe’s five component second- degree polynomial. The model was used to optimize the compressive strength of concrete made from, cement, sawdust ash, sand, granites and water. A total of ninety (90) cubes were cast, comprising of three cubes for each mix ratio of a total of thirty (30) mix ratios. The first fifteen (15) were used to determine the coefficients of the response function, while the other fifteen were used to validate the response function. The results from the response function compared favourably with the experimental results. The response function were tested with the statistical student’s t-test and found to be adequate at 95% confidence level. With the response function developed in this work, any desired compressive strength of sawdust ash-cement concrete can be predicted from known mix proportions and vice versa. Keywords: compressive strength, saw-dust ash, cement, concrete, Osadebe’s regression functions.

1.

Introduction

Majority of housing units and infrastructural facilities in Nigeria are constructed using concrete. Amongst the basic constituent of concrete, aggregates and cement are the most expensive, thus, the major determinant factors in the cost of producing concrete are cost of aggregates and cement. With the global economic recession coupled with the market inflationary trends, the constituent materials used for these structures had led to a very high cost of construction. Hence, researchers in material science and engineering are committed to having local materials to partially or fully replace these costly conventional materials. These local materials could be agricultural or industrial wastes. Some of these wastes include sawdust, pulverized fuel ash, palm kernel shells, slag, fly ash etc, which are produced from milling stations, thermal power station, waste treatment plants, etc. Numerous achievements have been made in these regards and the subject is attracting attention due to its functional benefit of waste reusability and sustainable development. Reduction in construction costs and the ability to produce light-weight structures, are added advantage. Sawdust can be defined as loose particles or wood chippings obtained as by-products from sawing of timber into standard useable sizes. Timber is one of the oldest structural materials used by man. Temples and monuments built several years ago, which still remain in excellent condition, show the durability and usefulness of timber (Kullkarni, 2005). Clean Sawdust without a large amount of bark, has proved to be satisfactory. This does not introduce a high content of organic material that may upset the reactions of hydration (Neville, 2000). It has pozzolanic properties and has been shown to react chemically with the calcium hydroxide released from the hydration of Portland cement, to form cement compounds (Elinwa and Mahmood, 2002). In this work, a mathematical model for the prediction and optimization of Compressive Strength of concrete is developed for concrete with different percentages of saw dust ash as partial replacement of cement. Compressive test of concrete with different mix ratios and percentages of sawdust ash was carried out in the laboratory. The results were used to develop Osadebe‟s regression mathematical response function. This response function would be used to predict the compressive strength of concrete given any mix ratio or predict mix ratios given a particular Compressive Strength of concrete.

II.

According to Osadebe(2003), concrete is a four- component composite produced by mixing water, cement, fine aggregate (sand) and coarse aggregate. These ingredients are mixed in reasonable proportions to

www.iosrjournals.org

73 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression achieve desired strength of the concrete. In this paper, the fifth component sawdust ash shall be added as one of the component materials of concrete. Let us consider an arbitrary amount â&#x20AC;&#x17E;Sâ&#x20AC;&#x; of a given concrete mixture and let the portion of the i th component of the five constituent materials of the concrete be Si, (where i= 1, 2, 3, 4, 5). This was carried out with the principle of absolute mass. Thus, đ?&#x2018;&#x2020;1 + đ?&#x2018;&#x2020;2 + đ?&#x2018;&#x2020;3 + đ?&#x2018;&#x2020;4 + đ?&#x2018;&#x2020;5 = đ?&#x2018;&#x2020;

(1)

where đ?&#x2018;&#x2020;1 , đ?&#x2018;&#x2020;2 , đ?&#x2018;&#x2020;3 , đ?&#x2018;&#x2020;4 đ?&#x2018;&#x17D;đ?&#x2018;&#x203A;đ?&#x2018;&#x2018; đ?&#x2018;&#x2020;5 are the quantities of water, cement, sawdust ash, Sand, and coarse aggregate. Dividing Eqn(1) through by đ?&#x2018;&#x2020;, gives: đ?&#x2018;&#x2020;1 đ?&#x2018;&#x2020;2 đ?&#x2018;&#x2020;3 đ?&#x2018;&#x2020;4 đ?&#x2018;&#x2020;5 + + + + =1 (2) đ?&#x2018;&#x2020; đ?&#x2018;&#x2020; đ?&#x2018;&#x2020; đ?&#x2018;&#x2020; đ?&#x2018;&#x2020; đ?&#x2018;&#x2020;đ?&#x2018;&#x2013; th where is the fractional proportion of the i constituent component of the concrete mixture. đ?&#x2018;&#x2020;

Let

đ?&#x2018;&#x2020;đ?&#x2018;&#x2013; đ?&#x2018;&#x2020;

= đ?&#x2018;?đ?&#x2018;&#x2013; ,

(3)

Substituting Eqn (3) into Eqn (2) yields: đ?&#x2018;?1 + đ?&#x2018;?2 + đ?&#x2018;?3 + đ?&#x2018;?4 + đ?&#x2018;?5 = 1

(4)

where đ?&#x2018;?1 , đ?&#x2018;?2 , đ?&#x2018;?3, đ?&#x2018;?4 and đ?&#x2018;?5 are fractional proportions of water, cement, sawdust ash, sand, and coarse aggregate respectively. In general, for any given concrete mixture, exists a vector Z (đ?&#x2018;?1 , đ?&#x2018;?2 , đ?&#x2018;?3, đ?&#x2018;?4 ). In this paper where five component materials are considered, the vector is transformed to Zi (đ?&#x2018;?1 , đ?&#x2018;?2 , đ?&#x2018;?3, đ?&#x2018;?4 , đ?&#x2018;?5 ) whose elements satisfy Eqn (4). Also, for each value of đ?&#x2018;?đ?&#x2018;&#x2013; , the following inequality holds: đ?&#x2018;?đ?&#x2018;&#x2013; > 0

(5)

It is important to note that the proportion of relative constituent ingredient of concrete govern the strength of the concrete at its hardened state. Thus, the compressive strength, Y, of concrete can be expressed mathematically using Eqn (6) as: Y = f (đ?&#x2018;?1 , đ?&#x2018;?2 , đ?&#x2018;?3, đ?&#x2018;?4 , đ?&#x2018;?5 )

(6)

where f (đ?&#x2018;?1 , đ?&#x2018;?2 , đ?&#x2018;?3, đ?&#x2018;?4 , đ?&#x2018;?5 ) is a multi-variate response function whose variables đ?&#x2018;?đ?&#x2018;&#x2013; are subject to the constraints defined in Eqns (4) and (5).

1.1 Osadebeâ&#x20AC;&#x2122;s regression equation This theory assumed that the response function is continuous and differentiable with respect to its variables, đ?&#x2018;?đ?&#x2018;&#x2013; , hence, it can be expanded using Taylorâ&#x20AC;&#x;s series in the neighbourhood of a chosen point đ?&#x2018;? 0 = đ?&#x2018;?10 + đ?&#x2018;?20 + đ?&#x2018;?30 + đ?&#x2018;?40 + đ?&#x2018;?50 as follows: đ?&#x2018;?đ?&#x2018;&#x2013; â&#x2C6;&#x2019; đ?&#x2018;? 0 đ?&#x2018;&#x201C; đ?&#x2018;? = đ?&#x2018;&#x201C;đ?&#x2018;&#x161; đ?&#x2018;? 0 + 7 đ?&#x2018;&#x161;! for

0â&#x2030;¤đ?&#x2018;&#x161;â&#x2030;¤â&#x2C6;&#x17E;

where m is the degree of polynomial of the response function and đ?&#x2018;&#x201C; đ?&#x2018;? is the response function. Expanding Eqn (7) to the second order yields:

www.iosrjournals.org

74 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression 5

đ?&#x2018;&#x201C; đ?&#x2018;? =đ?&#x2018;&#x201C; đ?&#x2018;?

(0)

+ đ?&#x2018;&#x2013;=1

+

đ?&#x153;&#x2022;đ?&#x2018;&#x201C; đ?&#x2018;? 0 đ?&#x153;&#x2022;đ?&#x2018;?đ?&#x2018;&#x2013;

1 ! 2

5

đ?&#x2018;&#x2013;=1

đ?&#x2018;?đ?&#x2018;&#x2013; â&#x2C6;&#x2019; đ?&#x2018;?đ?&#x2018;&#x2013;

2

đ?&#x153;&#x2022; đ?&#x2018;&#x201C; đ?&#x2018;? đ?&#x153;&#x2022;đ?&#x2018;?đ?&#x2018;&#x2013;2

0

1 + ! 2

0

4

5

đ?&#x2018;&#x2013;=1 đ?&#x2018;&#x2014; =1

đ?&#x153;&#x2022;2 đ?&#x2018;&#x201C; đ?&#x2018;? 0 đ?&#x153;&#x2022;đ?&#x2018;?đ?&#x2018;&#x2013; đ?&#x153;&#x2022;đ?&#x2018;?đ?&#x2018;&#x2014;

đ?&#x2018;?đ?&#x2018;&#x2013; â&#x2C6;&#x2019; đ?&#x2018;?đ?&#x2018;&#x2013;

0

đ?&#x2018;?đ?&#x2018;&#x2014; â&#x2C6;&#x2019; đ?&#x2018;?đ?&#x2018;&#x2014;

0

0

(đ?&#x2018;?đ?&#x2018;&#x2013; â&#x2C6;&#x2019; đ?&#x2018;?đ?&#x2018;&#x2013; )2 + â&#x2039;Ż

(8)

The point, đ?&#x2018;? 0 will be chosen as the origin for convenience sake without loss of generality of the formulation. The predictor, đ?&#x2018;?đ?&#x2018;&#x2013; is not the actual portion of the mixture component, rather, it is the ratio of the actual portions to the quantity of concrete. For convenience sake, let đ?&#x2018;?đ?&#x2018;&#x2013; be called the term of â&#x20AC;&#x153;fractional portionâ&#x20AC;?. The actual portions of the mixture components are Si. Consequently, the origin, Z(0) = 0, implies that: Z1(0)= 0, Z2(0)= 0, Z3(0)=0 , Z4(0)= 0, Z5(0)= 0 Let: đ?&#x2018;?0 = đ?&#x2018;&#x201C;(0) , đ?&#x2018;?đ?&#x2018;&#x2013; =

đ?&#x153;&#x2022;đ?&#x2018;&#x201C; (0)

đ?&#x153;&#x2022; 2 đ?&#x2018;&#x201C;(0)

đ?&#x153;&#x2022;đ?&#x2018;? đ?&#x2018;&#x2013;

đ?&#x153;&#x2022;đ?&#x2018;? đ?&#x2018;&#x2013; đ?&#x153;&#x2022;đ?&#x2018;? đ?&#x2018;&#x2014;

, đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2014; =

(9)

and đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2013; =

đ?&#x153;&#x2022; 2 đ?&#x2018;&#x201C;(0) đ?&#x153;&#x2022;đ?&#x2018;?đ?&#x2018;&#x2013;2

Then, Eqn (8) can be rewritten as follows:

5

đ?&#x2018;&#x201C; 0 = đ?&#x2018;?0 +

4

5

đ?&#x2018;?đ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2013; + đ?&#x2018;&#x2013;=1

5

đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2013;2 + â&#x2039;Ż

đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2014; đ?&#x2018;?đ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2014; + đ?&#x2018;&#x2013;=1 đ?&#x2018;&#x2014; =1

(10)

đ?&#x2018;&#x2013;=1

Multiplying Eqn (4) by b0, gives the following expression: b0 = b0Z1 + b0Z2 + b0 Z3 + b0Z4 + b0Z5

(11)

Similarly, multiplying Eqn (4) by Zi will yield the following expression: Z1 = Z12 + Z1 Z2+ Z1 Z3+ Z1 Z4+ Z1 Z5

(12a)

Z2 = Z1 Z2+ Z22+ Z2Z3+ Z2Z4+ Z2Z5

(12b)

Z3 = Z1 Z3+ Z2Z3+ Z33+ Z3Z4+ Z3Z5

(12c)

Z4= Z1 Z4+ Z2Z4 + Z4Z3+ Z42+ Z4Z5

(12d)

Z5 = Z1 Z5+ Z2Z5+ Z3Z5+ Z4Z5+ Z52

(12e)

When Eqns (12a) to (12e), are rearranged, the expression for Zi2 becomes; Z12 = Z1 - Z1Z2 - Z1Z3 - Z1Z4 - Z1Z5

(13a)

Z22 = Z2 - Z1Z2 â&#x20AC;&#x201C; Z2Z3 â&#x20AC;&#x201C; Z2Z4 â&#x20AC;&#x201C; Z2Z5

(13b)

Z32 = Z3 - Z1Z3 â&#x20AC;&#x201C; Z2Z3 â&#x20AC;&#x201C; Z3Z4 â&#x20AC;&#x201C; Z3Z5

(13c)

Z42 = Z4 - Z1Z4 â&#x20AC;&#x201C; Z2Z4 â&#x20AC;&#x201C; Z3Z4 â&#x20AC;&#x201C; Z4Z5

(13d)

Z52 = Z5 - Z1Z5 â&#x20AC;&#x201C; Z2Z5 â&#x20AC;&#x201C; Z3Z5 â&#x20AC;&#x201C; Z4Z5

(13e)

Substituting Eqn (13a) to (13e) into Eqn (10) and setting đ?&#x2018;&#x201C; 0 = đ?&#x2018;&#x152; give the expanded form below: www.iosrjournals.org

75 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression Y = b0Z1 + b0Z2 + b0Z3 + b0Z4 + b0Z5 + b1Z1 + b2Z2 + b3Z3 + b4Z4 + b5Z5+b12Z1Z2+ b13Z1Z1Z3 + b14Z1Z4 + b15Z1Z5 + b23Z2Z3 + b24Z2Z4+b25Z2Z5 + b34Z3Z4 + b35Z3Z5 + b45Z4Z5 + b11 (Z1 - Z1Z2 - Z1Z3 - Z1Z4 - Z1Z5 ) + b22 (Z2 â&#x20AC;&#x201C; Z1Z2 â&#x20AC;&#x201C; Z2Z3â&#x20AC;&#x201C; Z2Z4 â&#x20AC;&#x201C; Z2Z5) + b33 (Z3 â&#x20AC;&#x201C; Z1Z3 - Z2Z3 - Z3Z4 - Z3Z5) + b44 (Z4â&#x20AC;&#x201C; Z1Z4 - Z2Z4 - Z3Z4- Z4Z5 ) â&#x20AC;&#x201C; b55 (Z5 -Z1Z5 â&#x20AC;&#x201C; Z2Z5 â&#x20AC;&#x201C; Z3Z5â&#x20AC;&#x201C; Z4Z5 )

(14a)

Factorizing Eqn (14a) gives đ?&#x2018;&#x152; = đ?&#x2018;?1 đ?&#x2018;?0 + đ?&#x2018;?1 + đ?&#x2018;?11 + đ?&#x2018;?2 đ?&#x2018;?0 + đ?&#x2018;?2 + đ?&#x2018;?22 + đ?&#x2018;?3 đ?&#x2018;?0 + đ?&#x2018;?3 + đ?&#x2018;?33 + đ?&#x2018;?4 đ?&#x2018;?0 + đ?&#x2018;?4 + đ?&#x2018;?44 + đ?&#x2018;?5 đ?&#x2018;?0 + đ?&#x2018;?5 + đ?&#x2018;?55 + đ?&#x2018;?1 đ?&#x2018;?2 đ?&#x2018;?12 â&#x2C6;&#x2019; đ?&#x2018;?11 â&#x2C6;&#x2019; đ?&#x2018;?22 + đ?&#x2018;?1 đ?&#x2018;?3 đ?&#x2018;?13 â&#x2C6;&#x2019; đ?&#x2018;?11 â&#x2C6;&#x2019; đ?&#x2018;?33 + đ?&#x2018;?1 đ?&#x2018;?4 đ?&#x2018;?14 â&#x2C6;&#x2019; đ?&#x2018;?11 â&#x2C6;&#x2019; đ?&#x2018;?44 + đ?&#x2018;?1 đ?&#x2018;?5 đ?&#x2018;?15 â&#x2C6;&#x2019; đ?&#x2018;?11 â&#x2C6;&#x2019; đ?&#x2018;?55 + đ?&#x2018;?2 đ?&#x2018;?3 đ?&#x2018;?23 â&#x2C6;&#x2019; đ?&#x2018;?22 â&#x2C6;&#x2019; đ?&#x2018;?33 + đ?&#x2018;?2 đ?&#x2018;?4 đ?&#x2018;?24 â&#x2C6;&#x2019; đ?&#x2018;?22 â&#x2C6;&#x2019; đ?&#x2018;?44 + đ?&#x2018;?2 đ?&#x2018;?5 đ?&#x2018;?25 â&#x2C6;&#x2019; đ?&#x2018;?22 â&#x2C6;&#x2019; đ?&#x2018;?55 + đ?&#x2018;?3 đ?&#x2018;?4 đ?&#x2018;?34 â&#x2C6;&#x2019; đ?&#x2018;?33 â&#x2C6;&#x2019; đ?&#x2018;?44 + đ?&#x2018;?3 đ?&#x2018;?5 đ?&#x2018;?35 â&#x2C6;&#x2019; đ?&#x2018;?33 â&#x2C6;&#x2019; đ?&#x2018;?55 + đ?&#x2018;?4 đ?&#x2018;?5 đ?&#x2018;?45 â&#x2C6;&#x2019; đ?&#x2018;?44 â&#x2C6;&#x2019; đ?&#x2018;?55 (14đ?&#x2018;?) The summation of the constants is equal to a constant thus; let â&#x2C6;?đ?&#x2018;&#x2013; = đ?&#x2018;?0 + đ?&#x2018;?đ?&#x2018;&#x2013; + đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2013; đ?&#x2018;&#x17D;đ?&#x2018;&#x203A;đ?&#x2018;&#x2018; â&#x2C6;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2014; = đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2014; + đ?&#x2018;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2013; + đ?&#x2018;?đ?&#x2018;&#x2014;đ?&#x2018;&#x2014;

(15)

Eqn (14b) becomes: Y = â&#x2C6;?1Z1 + â&#x2C6;?2Z2 + â&#x2C6;?3Z3 + â&#x2C6;?4Z4 + â&#x2C6;?5Z5+ â&#x2C6;?12Z1Z2+ â&#x2C6;?13Z1Z3 + â&#x2C6;?14Z1Z4+ â&#x2C6;?15Z1Z5+ â&#x2C6;?23Z2Z3+ â&#x2C6;?24Z2Z4 + â&#x2C6;?25Z2Z5 + â&#x2C6;?34Z3Z4+ â&#x2C6;?35Z3Z5+ â&#x2C6;?45Z4Z5 (16a) Rewriting Eqn (16a) in a compact form, gives: 5

đ?&#x2018;&#x152;=

5

đ?&#x203A;źđ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2013; + đ?&#x2018;&#x2013;=1

đ?&#x203A;źđ?&#x2018;&#x2013;đ?&#x2018;&#x2014; đ?&#x2018;?đ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2014;

(16đ?&#x2018;?)

1â&#x2030;¤đ?&#x2018;&#x2013;â&#x2030;¤đ?&#x2018;&#x2014;

And, Y is the response function at any point of observation, đ?&#x2018;?đ?&#x2018;&#x2013; and đ?&#x2018;?đ?&#x2018;&#x2014; are the predictors, and â&#x2C6;?đ?&#x2018;&#x2013; and â&#x2C6;?đ?&#x2018;&#x2013;đ?&#x2018;&#x2014; are the coefficients of the response equation.

1.2 The Coefficients of the Regression Equation Let the nth response (compressive strength at nth observation point) be Y (n) and the vector of the corresponding set of variables be as follows: Z(n) = ( Z1(n), Z2(n), Z3(n), Z4(n), Z5(n)) Different points of observation will have different predictor at constant coefficient. At n th observation point, the response function, Y (n) , will correspond with the predictors Zi(n). Thus, 5

đ?&#x2018;&#x152;

(đ?&#x2018;&#x203A;)

5

(đ?&#x2018;&#x203A;) đ?&#x203A;źđ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2013;

= đ?&#x2018;&#x2013;=1

(đ?&#x2018;&#x203A;)

+

đ?&#x203A;źđ?&#x2018;&#x2013;đ?&#x2018;&#x2014; đ?&#x2018;?đ?&#x2018;&#x2013; đ?&#x2018;?đ?&#x2018;&#x2014;

(16)

1â&#x2030;¤đ?&#x2018;&#x2013;â&#x2030;¤đ?&#x2018;&#x2014;

where 1â&#x2030;¤ iâ&#x2030;¤ jâ&#x2030;¤ 5 and n= 1, 2, 3,â&#x20AC;Ś, 15 Eqn (16) can be rewritten in a matrix form as, [Y (n)] = [Z (n)] [â&#x2C6;?] Expanding Eqn (17) yields:

(17)

The actual mixture proportions Si (n) and the corresponding fractional portions, Zi(n) are shown in Table 1. And the values of the constant coefficient â&#x2C6;? in Eqn (17), are determined with the values of Y(n) and Z(n). Rearranging Eqn (17) gives www.iosrjournals.org

76 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression [â&#x2C6;?] = [Z(n)]-1 [Y(n)]

(19)

Expressing Eqn. (19) in expanded form yields:

The values of â&#x2C6;?1 to â&#x2C6;?45 are obtained from Eqn (20) and substituted into Eqn. (16a) to obtain the regression equation. The values of Z (n)] matrix are shown in Table 2 and the values of the inverse of [Z (n)] matrix are presented in Table 3; while the values of [Y (n)] matrix are obtained from the experimental investigation.

III. III.1

Materials and Methods

Materials

The materials used for the laboratory test included: (i) Water that is good for drinking obtained from a borehole at the premises of Federal University of Technology Owerri, Imo State, Nigeria. The water was clean, fresh and free from dirt, unwanted chemicals or rubbish that may affect the desired quality of concrete. (ii) Dangote cement, a brand of ordinary Portland cement that conforms to BS 12(1978) (iii) The fine aggregate, river sand used for this research work were obtained from a flowing river (Otamiri). As at the time of purchase the sharp river sand was wet but free from debris and deleterious matter and clay. (iv) The coarse aggregate used for this research work was granite chippings quarried from a quarry in Ishiagu, along Enugu-Port Harcourt express way, a town in Ebonyi state, Nigeria. The granite was sun dried for seven days so they can be free from water. They were sieved through a 20mm British test sieve and the materials passing through the sieve were used to produce concrete with various proportions of termite soil. (v) Sawdust is a by-product from timber, it is a waste product obtained during sawing of timber into standard sizes. The sawdust was obtained from timber milling market (ogbosisi) Owerri. This material was first dried to remove the natural moisture. The waste was burnt in an enclosure (i.e. open drum) at temperature of about 400-500Â°C to obtain sawdust ash. The ash was allowed to cool; thereafter the ash was sieved with 150Îźm sieve aperture to obtain the finest particle of material which approximates to the fineness of that of cement used. The mix ratios used for the laboratory test, were obtained using pentahedron factor space for five â&#x20AC;&#x201C; component mixture.

3.2 Compressive Strength Test Batching of the ingredients was done by mass. A mixture of Cement/ sawdust ash was thoroughly mixed together in the dry state river sand and granite and then, water added. The mixing continued until a uniform and consistent concrete mix is obtained. The entire concrete was cast in concrete mould of sizes 150 x 150x 150 mm. In all, sixty concrete cubes, two from each mix incorporating various proportions of sawdust ash, were cast and cured in a curing water tank for 28 days, and then crushed in a universal testing machine. Thirty of the concrete cubes served as control test. Compressive strength of the cubes was calculated using Eqn (21): Compressive strength =

đ?&#x2018;?đ?&#x2018;&#x153;đ?&#x2018;&#x161;đ?&#x2018;?đ?&#x2018;&#x;đ?&#x2018;&#x2019;đ?&#x2018; đ?&#x2018; đ?&#x2018;&#x2013;đ?&#x2018;Łđ?&#x2018;&#x2019; đ?&#x2018;&#x2122;đ?&#x2018;&#x153;đ?&#x2018;&#x17D;đ?&#x2018;&#x2018; đ?&#x2018;&#x153;đ?&#x2018;&#x201C; đ?&#x2018;?đ?&#x2018;˘đ?&#x2018;?đ?&#x2018;&#x2019; đ?&#x2018;&#x17D;đ?&#x2018;Ą đ?&#x2018;&#x201C;đ?&#x2018;&#x17D;đ?&#x2018;&#x2013;đ?&#x2018;&#x2122;đ?&#x2018;˘đ?&#x2018;&#x;đ?&#x2018;&#x2019; (đ?&#x2018; ) đ?&#x2018;?đ?&#x2018;&#x;đ?&#x2018;&#x153;đ?&#x2018; đ?&#x2018;  đ?&#x2018; đ?&#x2018;&#x2019;đ?&#x2018;?đ?&#x2018;Ąđ?&#x2018;&#x2013;đ?&#x2018;&#x153;đ?&#x2018;&#x203A;đ?&#x2018;&#x17D;đ?&#x2018;&#x2122; đ?&#x2018;&#x17D;đ?&#x2018;&#x;đ?&#x2018;&#x2019;đ?&#x2018;&#x17D; đ?&#x2018;&#x153;đ?&#x2018;&#x201C; đ?&#x2018;&#x161;đ?&#x2018;&#x153;đ?&#x2018;˘đ?&#x2018;&#x2122;đ?&#x2018;&#x2018; (đ?&#x2018;&#x161; đ?&#x2018;&#x161; 2 )

(21)

The results of the compressive strength test of the concrete cubes are presented in Table 4

www.iosrjournals.org

77 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression Table 1: Selcted mix proportions, S, and their corresponding fractional portions,Z, based on Osadebeâ&#x20AC;&#x2122;s second-degree polynomial Mix Proportions, đ?&#x2018;şđ?&#x2019;&#x160;

FractionaL Portions, đ?&#x2019; đ?&#x2019;&#x160;

OP 1

S1 0.5

S2 0.95

S3 0.05

S4 2.25

S5 4.00

Z1 0.065

Z2 0.123

Z3 0.006

Z4 0.290

Z5 0.516

2 S3 4 5 12 13 14 15 23 24 25 34 35 45

0.55 0.60 0.45 0.05 0.525 0.55 0.475 0.575 0.575 0.50 0.60 0.525 0.625 0.55

0.90 0.15 0.80 0.75 0.925 0.90 0.875 0.85 0.875 0.85 0.825 0.825 0.80 0.775

0.10 0.15 0.20 0.25 0.075 0.10 0.125 0.150 0.125 0.150 0.175 0.175 0.20 0.225

175 2.25 1.50 2.50 2.00 2.25 1.875 2.375 2.00 1.625 2.125 1.875 2.375 2.00

3.50 4.25 3.00 5.00 3.75 4.125 3.50 4.50 3.875 3.25 4.25 3.625 4.625 4.00

0.0809 0.0741 0.0710 0.0710 0.0722 0.069 0.069 0.0680 0.0772 0.0784 0.0752 0.0747 0.0725 0.0728

0.1323 0.10493 0.1344 0.081967 0.0227 0.1136 0.128 0.1006 0.1175 0.1333 0.1034 0.1174 0.0928 0.1026

0.0147 0.0185 0.0336 0.0273 0.0103 0.0126 0.0182 0.0178 0.0168 0.0235 0.02194 0.0249 0.0232 0.0298

0.2514 0.2778 0.252 0.273 0.2749 0.2839 0.2737 0.2811 0.2685 0.2549 0.2665 0.2669 0.2754 0.2649

0.5147 0.525 0.504 0.546 0.5155 0.5210 0.5109 0.5325 0.5200 0.5098 0.5329 0.5160 0.5362 0.5298

CONTROL POINTS AC1 0.550 0.900 0.100 2.083 AC2 0.517 0.867 0.133 2.000 AC3 0.533 0.833 0.167 2.083 AC4 0.525 0.875 0.125 1.938 AC5 0.550 0.838 0.163 2.125 AC6 0.575 0.863 0.138 2.188 AC7 0.538 0.913 0.088 2.125 AC8 0.600 0.825 0.175 2.375 AC9 0.520 0.890 0.110 2.000 AC10 0.550 0.850 0.150 2.050 AC11 0.545 0.855 0.145 2.100 AC12 0.545 0.835 0.165 1.975 AC13 0.570 0.868 0.133 2.238 AC14 0.545 0.855 0.145 2.050 AC15 0.538 0.858 0.143 2.150 Legend: OP is Observation Point

3.917 3.750 4.000 3.688 4.063 4.183 3.938 4.563 3.750 3.950 4.000 3.850 4.238 3.938 4.075

0.073 0.071 0.070 0.073 0.071 0.072 0.071 0.070 0.072 0.073 0.071 0.074 0.071 0.072 0.069

0.119 0.119 0.109 0.122 0.108 0.109 0.120 0.097 0.122 0.113 0.112 0.113 0.108 0.114 0.110

0.013 0.018 0.022 0.017 0.021 0.017 0.012 0.020 0.015 0.020 0.019 0.022 0.016 0.019 0.018

0.276 0.275 0.274 0.271 0.275 0.275 0.280 0.278 0.275 0.272 0.275 0.268 0.278 0.272 0.277

0.519 0.516 0.525 0.516 0.525 0.526 0.518 0.534 0.516 0.523 0.523 0.522 0.527 0.523 0.525

www.iosrjournals.org

78 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression

www.iosrjournals.org

79 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebe’s Regression IV.

Results And Analysis

The sawdust ash-cement concrete cubes, were crushed on the 28th day, and the results presented in table 4 Table 4: Compressive strength in N/mm2 of 28th day old concrete cubes

4.2 The final response function The solution of Eqn (20),using the responses in Table 4 and the Z matrix, gives the unknown coefficients of the regression equation as follows: 1 = 178559.1 2 = 15572.47 3 = -2689.94 4 = 3939.83 5 = 1699.999 12 = -329399 13 = -218425 14 = -91088.2 15 = -246507 23 = -35766.2 24 = 649779.6 25 = 19521.98 34 = -41692.3 35 = 32895.84 45 = -11530.2 Substituting these coefficients into Eqn. (16a) yields: Y = 178559.1Z1 + 15572.47Z2 – 2689.94Z3 + 3939.83Z4 + 1699.999Z5 – 329399Z1Z2 – 1218425Z1Z3 – 91088.2Z1Z4 – 246507Z1Z5 – 35766.2Z2Z3 – 64979.6Z2Z4 + 19521.98Z2Z5 – 41692.3Z3Z4 + 32895.84Z3Z5 – 11530.20Z4Z5 (22) The Eqn (22), is the final response function for the predicting of the compressive strength of sawdust ashcement concrete based on Osadebe‟s regression function.

www.iosrjournals.org

80 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebeâ&#x20AC;&#x2122;s Regression 4.3 Test of Adequacy of the response function

The test for adequacy of response function was done using two-tailed statistical studentâ&#x20AC;&#x;s t-test at 95% accuracy level. The compressive strengths at the control points (i.e. AC1, AC2 , AC3 ,AC4, AC5, AC6 ,AC7, AC8 ,AC9 ,AC10, AC11, AC12, AC13, AC14, AC15) were used for the test . The following two hypotheses were tested using statistical studentâ&#x20AC;&#x;s t-test. a) Null Hypothesis: There is no significant difference between the laboratory concrete cube strengths and predicted compressive strength results at 95% accuracy level. b) Alternative Hypothesis: There is a significant difference between the laboratory concrete cube strengths and l predicted strength compressive strength results at 95% accuracy level. The test is carried out and presented in Table 5 using the following equations: where YE = Responses compressive strength from the experiment YM = Responses(compressive strength) from the Second degree polynomial equation N = Number of observations points Di = Difference of YE and YM Di DA = =Mean of difference of YE and YM S2 = t =

đ?&#x2018; (D A â&#x20AC;&#x201C; Di )2 Nâ&#x2C6;&#x2019;1 D A â&#x2C6;&#x2014;N 0.5 S

= Variance of difference of Di and DA = Calculated value of t

Table 5: Statistical Studentâ&#x20AC;&#x2122;s t-test for Osadebeâ&#x20AC;&#x2122;s response function OP AC1 AC2 AC3 AC4 AC5 AC6 AC7 AC8 AC9 AC10 AC11 AC12 AC13 AC14 AC15

YE 17.48 14.74 15.58 16.45 14.17 14.67 17.14 11.48 16.39 14.30 13.50 14.80 13.05 14.58 13.11

YM 15.98 13.24 14.51 14.95 13.67 14.17 16.14 11.43 15.39 14.80 14.00 15.50 13.20 14.76 13.81 ď &#x201C;ď &#x201C;Di =

Di =YE - YM

DA - đ??ˇđ?&#x2018;&#x2013;

(DA - đ??ˇđ?&#x2018;&#x2013; )2

1.50 1.50 1.07 1.50 0.50 0.50 1.00 0.05 1.00 -0.50 -0.50 -0.70 -0.15 -0.18 -0.70

-1.107 -1.107 -0.677 -1.107 -0.107 -0.107 -0.607 0.343 -0.607 0.893 0.893 1.093 0.543 0.573 1.093

1.2254 1.2254 0.4583 1.2254 0.0114 0.0114 0.3684 0.1176 0.3684 0.7974 0.7974 1.1946 0.2948 0.3283 1.1946

5.89

ď &#x201C;ď &#x201C;(DA- Di)2 =

9.6191

Here, ď &#x201C;ď &#x201C;Di = 5.89Legend: OP is the observation point N = 15 đ??ˇ DA = đ?&#x2018; đ?&#x2018;&#x2013; = 0.393 S2 =

(D A â&#x20AC;&#x201C; D i )2

= 0.6871

N â&#x2C6;&#x2019;1 đ?&#x2018;&#x2020; 2 = 0.8289

S= The actual value of the total variation in t-test is given by DA â&#x2C6;&#x2014;N 0.5

t = = 1.84 S and the allowable value of the total variation in t-test is obtained as follows Degree of freedom = N-1 = 15-1 = 14 5 % significance for Two-Tailed Test = 2.5 % 1 - 2.5% = 97.5% = 0.975 Therefore allowable total variation in the t-test = t (0.975, N-1) = t (0.975, 14) = 2.14 (Obtained from standard www.iosrjournals.org

81 | Page

Prediction Of Compressive Strength Of Sawdust Ash- Cement Concrete Using Osadebe’s Regression statistical table). From table 5, the calculated t = 1.84 Thus, t(table) > t(calculated) This implied that difference between the two set of cubes compressive strength is less than allowable difference. Hence null hypothesis is accepted and alternative hypothesis rejected. Hence, Osadebe regression model is adequate.

V.

Conclusion

Using Osadebe‟s second degree polynomial regression equation, mix design model for a five component sawdust ash-cement concrete. This model could predict the compressive strength of concrete cube when the mix ratios are known and vice versa. The predictions from this model were tested at 95% accuracy level using statistical student‟s t-test and found to be adequate.

References [1] [2] [3] [4] [5] [6] [7] [8] [9]

Afolayan, J.O. and Alhassan , A.Y. (2010) “Durability of Concrete Containing Fly Ash in Aggressive Environment” . Journals of Engineering and Applied Science. Vol. 2 BS 12: (1978), “Specification for Portland cement”. Elinwa, A.U. and Mahmood, Y. A. (2002). “Ash from timber waste as cement replacement material. Cement and Concrete Composites, 24, 219 – 222. Elinwa, A.U. and Abdulkadir, S. (2011) “Characterizing Sawdust ash for Use as an inhibitor for Reinforcement Corrosion.” New Clues in Science. 1-10 Neville, A.M., (1996), “Properties of Concrete”, Longman Ltd., England Neville, A.M., and Brook, J.J.,( 1990), “Concrete Technology”, Longman Ltd., Singapore Scheffe, H. (1958), “Experiments with Mixtures”, Journal of the Royal Statistical Society. Ser. B., 20, 344 – 360. Obam, S.O.(2009). “A mathematical model for Optimization of Strength of Concrete: A case study for shear modulus of Rice Husk Ash Concrete. Journal of Industrial Engineering International. Vol.5 (9) 76-84 Osadebe, N.N., (2003). “Generalized Mathematical Modelling of Compressive Strength of Normal Concrete as Multi-variate function of the Properties of its Constituents components”. A paper delivered at college of Engineering, University of Nigeria Nsukka.

www.iosrjournals.org

82 | Page

Prediction of Compressive Strength of Sawdust Ash- Cement Concrete Using Osadebe’s Regression Funct

http://www.iosrjournals.org/iosr-jmce/papers/vol6-issue1/J0617382.pdf